In situ determination of aging precipitation in deformed Fe-Cu and Fe-Cu-B-N alloys
by time-resolved small-angle neutron scattering
S. M. He,1,
*N. H. van Dijk,1M. Paladugu,1 H. Schut,2J. Kohlbrecher,3 F. D. Tichelaar,4and S. van der Zwaag5 1Fundamental Aspects of Materials and Energy, Faculty of Applied Sciences, Delft University of Technology, Mekelweg 15,
2629 JB Delft, The Netherlands
2Neutron and Positron Methods in Materials, Faculty of Applied Sciences, Delft University of Technology, Mekelweg 15, 2629 JB Delft, The Netherlands
3Laboratory for Neutron Scattering, ETHZ and PSI, CH-5232 Villigen PSI, Switzerland
4Kavli Institute of Nanoscience, National Centre for HREM, Delft University of Technology, Lorentzweg 1, 2628 CJ Delft, The Netherlands
5Novel Aerospace Materials, Faculty of Aerospace Engineering, Kluyverweg 1, 2629 HS Delft, The Netherlands 共Received 4 August 2010; revised manuscript received 13 October 2010; published 12 November 2010兲 We performed in situ time-resolved small-angle neutron scattering共SANS兲 measurements on high-purity Fe-Cu and Fe-Cu-B-N alloys during isothermal aging at 550 ° C in order to study the potential self-healing of deformation-induced defects by nanosized Cu precipitation. Three different samples with 0%, 8%, and 24% prestrain were used to study the influence of variable defect levels on the Cu precipitation kinetics. The time-resolved SANS measurements show the presence of two contributions corresponding to spherical pre-cipitates and precipitation at dislocations and/or interfaces, as confirmed by complementary transmission elec-tron microscopy experiments. For the Fe-Cu alloy, prestrain was found to accelerate the formation of spherical precipitates in initial aging stage and lead to a significant enhancement of copper precipitation at dislocations and/or interfaces. For the Fe-Cu-B-N alloy, the addition of boron and nitrogen accelerates the formation of spherical precipitates but suppresses the precipitation along dislocations in the prestrained samples.
DOI:10.1103/PhysRevB.82.174111 PACS number共s兲: 61.66.Dk, 61.72.⫺y, 64.75.Op, 61.05.fg
Steels are among the most widely used construction ma-terials as their mechanical properties can be tailored to obtain the required combination of strength and formability. How-ever, in highly demanding applications the lifetime until fail-ure of steels is limited due to the accumulation of damage, ultimately leading to the formation of ultrafine cracks that subsequently grow and ultimately cause fracture of the steel components.
Recently it was recognized that in aluminum alloys1 and
steels2,3the growth of ultrafine cracks can be immobilized in
an early stage by the dynamic formation of nanoscale pre-cipitates. This process is known as self-healing and can sig-nificantly enhance the lifetime of structural components. So far, relatively little research has been done on self-healing in metals.4 For austenitic stainless steels,2,3dynamic precipita-tion of both Cu and BN was found to reduce creep damage under a load at high temperatures. The precipitates are as-sumed to partly fill the nanoscale open volume defects and thereby prevent their further growth.
In order to fully understand the role of these alloying elements and the influence of thermomechanical processing on the defect-induced precipitation, responsible for self-healing, additional studies on less complex low-alloyed steel grades are desirable. Therefore, high-purity Cu and Fe-Cu-B-N model alloys have been prepared in order to identify the physical mechanism responsible for self-healing in fer-ritic steels 关with a body-centered-cubic 共bcc兲 matrix兴. This insight will then make it possible to successfully introduce these concepts in industrial steel grades.
The precipitation of copper from supersaturated Fe-Cu alloys has been investigated extensively, both
experimentally5–20and theoretically.21–24It is now generally
accepted that, in the initial stage, fully coherent Cu precipi-tates inherit the bcc structure of the ␣-Fe matrix. When reaching a critical diameter of approximately 4–6 nm, the growing bcc precipitates undergo a martensitic transforma-tion to a less coherent 9R structure. At sizes larger than 15–17 nm, a second transformation to the more stable 3R structure takes place before the Cu precipitates adopt their equilibrium face-centered-cubic 共fcc兲 structure. The full transformation sequence for copper precipitation in Fe-Cu alloys is given by bcc→9R→3R→fcc for increasing aging time. As far as the composition of Cu precipitates is con-cerned, the Cu precipitates are almost pure Cu at sizes above 4–5 nm but there exists contradicting information about their composition during the initial stage of the precipitation pro-cess. Investigations performed with atom probe analysis con-sistently report that the early Cu precipitates contain a sig-nificant fraction of Fe 共in some cases even in excess of 50 at. %兲,9–12which was later supported by thermodynamic
calculations.24The probe analysis, nevertheless, can generate
a large statistical error and underestimate the solute concen-tration in small precipitates due to the finite probe resolution. In contrast, results obtained with small-angle neutron scatter-ing共SANS兲 共Refs.13–16兲 and positron annihilation17–20 sug-gest that the precipitates are almost pure Cu with only minor amounts of Fe. Interpretation of the latter experiments de-pends however on a priori knowledge of the physical prop-erties of the small Cu clusters, which may cause some un-certainty in the determination of the composition of the Cu precipitates in the initial stage of the precipitation process. The composition of the metastable ultrafine bcc Cu precipi-tates in the Fe-Cu system is therefore still an open question.
More theoretical and experimental investigations are needed to solve this controversy.
In order to unravel the mechanism responsible for self-healing in steels it is essential to obtain detailed information on 共i兲 the influence of open-volume defects 共vacancies, va-cancy clusters, and dislocations兲 and 共ii兲 microalloying with B and N on the Cu precipitation kinetics in Fe-Cu alloys, which is currently not available. It is well known that open-volume defects facilitate the diffusion of solutes and thereby accelerate the precipitation, which is expected to promote the self-healing of metals by dynamic precipitation. Disloca-tions, which are easily multiplied by deformation, are found to accelerate the diffusion of impurities by almost three or-ders of magnitude compared to bulk diffusion25 and have
been proposed to play a role as heterogeneous nucleation sites for Cu precipitation.26The addition of boron and
nitro-gen was found to suppress creep cavity growth in copper-containing stainless steels, leading to a higher rupture strength and rupture ductility.3The effect of boron and nitro-gen on the copper precipitation mechanism has so far not been clarified.
Although the Cu precipitation kinetics of Fe-Cu has been investigated in earlier SANS 共Refs. 13–16 and 27兲 and small-angle x-ray scattering 共SAXS兲 experiments,28,29 lim-ited information is available on the precipitation behavior before peak aging. Previous SANS and SAXS experiments were all performed ex situ共at room temperature兲 and neither concentrate on the effect of deformation on the Cu precipi-tation nor on the addition of B and N.
In order to establish the potential of self-healing of de-fects by dynamic precipitation and to reach a detailed under-standing of the influence of both deformation and added bo-ron and nitrogen on the Cu precipitation in ibo-ron-based alloys, we performed in situ time-resolved SANS measurements on predeformed high-purity Fe-Cu and Fe-Cu-B-N alloys dur-ing isothermal agdur-ing at high temperatures. These time-resolved SANS measurements provide valuable information on the evolution of the precipitate size distribution. For com-parison, complementary hardness tests and transmission electron microscope 共TEM兲 observations have been per-formed. The results are compared to earlier positron annihi-lation spectroscopy measurements30 performed on the same
II. EXPERIMENTAL METHODS A. Material, heat treatments, and hardness tests
The chemical composition of the studied high-purity Fe-Cu and Fe-Cu-B-N alloys is listed in TableI. Both alloys
were produced by Goodfellow as a rolled sheet with a thick-ness of 0.5 mm. From this material dog-bone 共I兲 shaped samples were cut by spark erosion for tensile deformation tests. The samples were solution treated at 850 ° C for 1 h in evacuated silica tubes filled with 200 mbar ultrahigh-purity argon gas and subsequently quenched into water at room temperature. This solution treatment resulted in a fully equi-axed ferritic structure with a grain size of approximately 60 m. Part of the as-quenched samples were subjected to tensile deformation at room temperature up to a strain of 8% or 24% using a 2 kN microtensile tester 共Deben兲 with an initial slow strain rate of 2.67⫻10−4 s−1.
Hardness test were performed on samples that were aged for 0–100 h at 550 ° C in a salt bath. For the hardness tests a Buehler microhardness tester was used with a Vickers micro-hardness indenter, a load of 4.9 N and a holding time of 15 s.
B. Small-angle neutron scattering
In order to study the self-healing mechanism of defects by the formation of nanosized Cu precipitates and the role of added boron and nitrogen in copper-based iron alloys, time-resolved SANS measurements on the Fe-Cu and Fe-Cu-B-N alloys were carried out on the instrument SANS-I at PSI, Switzerland. These experiments were performed on the alloy samples during 12 h of aging at a constant temperature of 550 ° C in a vacuum chamber 共⬍10−2 Pa兲 to monitor the precipitation kinetics of Cu precipitates in: 共a兲 undeformed and plastically predeformed samples with 共b兲 8% and 共c兲 24% strain. The applied heating rate at the start of the ex-periments was of 73 ° C/min 共1.2 °C/s兲. The in situ SANS measurements were performed with a neutron wavelength of =0.7 nm 共⌬/=10%兲 at sample-to-detector distances of 2, 6, and 18 m 共longest distance was only used before and after aging兲. During aging at 550 °C time-resolved measure-ments SANS were performed by continuously switching the sample-to-detector distance between 2 and 6 m. The expo-sure time at each position was 150 s for the first hour and 300 s afterward. A transverse magnetic field of 1.1 T was applied perpendicular to the incident neutron beam in order to separate the nuclear共isotropic兲 and magnetic 共anisotropic兲 scattering.
C. Transmission electron microscopy
Disks for transmission electron microscopy were prepared by mechanical grinding down to 80 m. The thin foils were then etched in a Tenupol jet polisher with a 5% perchloric acid—95% acetic acid solution, held at 15 ° C using a volt-age of 35 V. Microscopy was carried out using a Philips CM30T operating at 300 kV and a Tecnai F20STEM/ST op-erating at 200 kV. Image analysis was conducted on two samples with 0% and 8% prestrain which have been mea-sured by SANS at 550 ° C for 12 h.
III. RESULTS A. Aging curves
In Fig.1, the effect of aging at 550 ° C on the hardness is shown for the as-quenched Fe-Cu and Fe-Cu-B-N alloys TABLE I. Chemical composition of the studied high-purity
model alloys共in wt %兲 with balance iron. The Ce content refers to the added nominal composition.
Alloy Cu B N C S Ce
Fe-Cu 1.11 ⬍0.01 0.002 0.0056 0.002 0.015
with and without 8% prestrain. For the undeformed alloys, the typical age-hardening behavior for copper precipitation is observed. The peak hardness is reached at about 6 h for the Fe-Cu alloy and 4 h for the Fe-Cu-B-N alloy. The 8% pre-strain leads to a significant increase in the initial hardness caused by cold-work hardening, which reduces during aging. The hardness of the deformed alloys with 8% prestrain de-creases in the initial aging stage due to the recovery of dis-locations, then rises quickly with aging in the regime from underaged to peak-aged, and finally decreases again in the overaged stage. For the Fe-Cu alloy, the hardness of the de-formed sample exceeds that of the undede-formed sample until the peak-aged regime is reached but seems to be lower than that of the undeformed sample in the overaged regime. For the Fe-Cu-B-N alloy, the hardness of the deformed sample is above that of undeformed sample in the peak-aged regime while the hardness of the deformed and undeformed samples is quite comparable in the underaged and overaged regime.
A comparison of the aging behavior of both alloys in Fig. 1 indicates that the Fe-Cu-B-N alloy has a faster response than the Fe-Cu alloy. This means that the precipitation of Fe-Cu alloy is accelerated by the addition of B and N. The time to peak hardness was found to be relatively insensitive to the predeformation: only for the Fe-Cu alloy the predefor-mation seems to result in a minor reduction in the time to peak hardness.
The results for the Fe-Cu alloy with 1.1 wt % Cu are in good agreement with earlier hardness studies on binary Fe-Cu alloys. Both the peak hardness and the aging time to peak are in between those reported for 0.8 wt % Cu 共Ref. 28兲 and for 1.3 wt % Cu.14The observed effect of prestrain
on the hardness during aging is consistent with that observed by Deschamps and co-workers.28
B. Small-angle neutron scattering
By applying a transverse magnetic field of 0H = 1.1 T, the magnetization of the ferromagnetic Fe-Cu alloy contain-ing nonmagnetic Cu clusters共fcc copper is weakly diamag-netic兲 is nearly saturated with the spins in the ferromagnetic matrix aligned along the magnetic field共x axis兲
perpendicu-lar to the incident neutron beam共z axis兲. Figure2shows the two-dimensional SANS patterns obtained for our Fe-Cu al-loy with 24% prestrain before and after isothermal aging for 12 h at 550 ° C. The data were recorded for a neutron wave-length of 7 Å at a sample-detector distance of 6 m. As shown in Fig.2共a兲, a weakly anisotropic scattering pattern is observed before aging with a dominant scattering contribu-tion perpendicular to the applied magnetic field. This aniso-tropy of the scattered intensity becomes more pronounced with increasing aging times. As shown in Fig. 2共b兲, a strongly anisotropic scattering pattern has formed after 12 h aging at 550 ° C. From the two-dimensional patterns the SANS cross section 共dd⍀⌺兲共Q兲 can be obtained, where Q =共Qx, Qy, 0兲 is the scattering vector with a wave-vector transfer Qxand Qy along the horizontal共x兲 and vertical 共y兲 axis, respectively. For a magnetically saturated sample the total SANS cross section can be expressed as a sum of both magnetic and nuclear scattering components,31
冉d⌺ d⍀冊MAGsin 2␣, 共1兲
where␣is the angle between applied magnetic field H 共ori-entation of the magnetization of the specimen M兲 and the scattering vector Q. The scattered intensity along 共␣= 0°兲 and perpendicular 共␣= 90°兲 to the applied magnetic field is expressed as 共d⌺/d⍀兲H储Q and 共d⌺/d⍀兲H⬜Q, respectively.
The nuclear共isotropic兲 and magnetic 共anisotropic兲 scattering components correspond to
冉d⌺ d⍀冊H储Q , 共2兲
冉d⌺ d⍀冊H⬜Q −
冊H储Q . 共3兲
Since the complete two-dimensional scattering pattern is measured, the magnetic and nuclear scattering components can be obtained simultaneously from a fit of the full scatter-ing pattern with Eq.共1兲. Figures3and4show the Q depen-dence of the nuclear 共isotropic兲 and magnetic 共anisotropic兲 scattering components for the Fe-Cu and Fe-Cu-B-N alloys
FIG. 1. 共Color online兲 Hardness aging curves of the as-quenched Fe-Cu and Fe-Cu-B-N samples aged at 550 °C with and without 8% predeformation.
with 0% and 24% prestrain before and after aging at 550 ° C for 12 h. The scattering intensities of the specimens with 8% prestrain are very similar to those for 24% prestrain. Before aging, the Fe-Cu alloy is fully solutionised and the SANS signal in Fig.3roughly follows a power-law behavior with a constant background for both the nuclear and the magnetic contributions 共with a minor additional contribution of
un-known origin centered around 0.1 nm−1兲. The additional scattering observed after aging is a result of the Cu precipi-tation. The data indicate that especially the magnetic scatter-ing is strongly enhanced by agscatter-ing. Without deformation, the additional contribution of the nuclear and magnetic scatter-ing caused by agscatter-ing has roughly the same Q dependence in the range 0.2⬍Q⬍2 nm−1, reflecting the formation of
FIG. 2.共Color online兲 Small-angle neutron-scattering patterns of the Fe-Cu alloy with 24% prestrain 共a兲 before and 共b兲 after 12 h of aging at 550 ° C. A magnetic field of 1.1 T was applied horizontally共along Qx兲.
FIG. 3.共Color online兲 Nuclear and magnetic SANS components as a function of the wave-vector transfer Q for the Fe-Cu alloy with 0% and 24% prestrain measured at room temperature before and after aging at 550 ° C for 12 h.
共spherical兲 nanoscale Cu precipitates. With 24% prestrain, a similar contribution is observed with a complementary in-crease in the power-law contribution for Q⬍0.1 nm−1in the nuclear scattering. This complementary nuclear contribution, observed for the deformed sample, reflects additional scatter-ing from Cu precipitation at more extended objects 共disloca-tions or interfaces兲.
For the Fe-Cu-B-N alloy 共Fig. 4兲, the aging response of the SANS signal shows a similar increase in nuclear and magnetic scattering in the range 0.2⬍Q⬍2 nm−1, reflecting the formation of nanoscale Cu precipitates. In contrast, the
increase in nuclear scattering at low Q 共Q⬍0.1 nm−1兲 is found to be much lower for the deformed Fe-Cu-B-N sample than for the deformed Fe-Cu sample after aging.
In order to monitor the time evolution during aging of the scattering from the nanoscale precipitates, we have evaluated the magnetic scattering by plotting共d⌺/d⍀兲MAGQ2versus Q for the Fe-Cu and Fe-Cu-B-N alloys with 0%, 8%, and 24% prestrain. In Fig.5共d⌺/d⍀兲MAGQ2versus Q is illustrated for the Fe-Cu alloys with 0% and 24% prestrain after subtraction of the initial scattering data from the as-quenched condition 共note that the data for Q⬍0.2 nm−1 have been suppressed兲.
FIG. 4.共Color online兲 Nuclear and magnetic SANS components as a function of the wave-vector transfer Q for the Fe-Cu-B-N alloy with 0% and 24% prestrain measured at room temperature before and after aging at 550 ° C for 12 h.
FIG. 5. 共Color online兲 Time evolution of 共d⌺/d⍀兲MAGQ2as a function of Q for the Fe-Cu alloys with共a兲 0% and 共b兲 24% prestrain during aging at 550 ° C up to 12 h after subtraction of the initial scattering data for the homogenized condition before aging.
A progressive increase in 共d⌺/d⍀兲MAGQ2 in the Q range 0.2– 2 nm−1 is observed with a maximum around 0.5 nm−1 for all the samples. The maximum was found to decrease with increasing prestrain. The volume fraction fV of nano-sized Cu particles can be evaluated by integrating the 共d⌺/d⍀兲MAGQ2 curve of magnetic scattering component.31 From the area under the共d⌺/d⍀兲Q2 curve for the magnetic 共nuclear兲 scattering, the magnetic 共nuclear兲 invariant Q0may be calculated, Q0,i=
冉d⌺ d⍀冊i Q2dQ = 22共⌬i兲2fV共1 − fV兲, 共4兲 where label i refers to the magnetic or nuclear SANS contribution, ⌬ is the difference in the magnetic共nuclear兲 scattering length density of the matrix and the precipitate. The magnetic scattering length density amounts to
MAG= N0p0 for the ferromagnetic matrix, where N0 is the number density of the magnetic moments, p0= 2.699 fm/B is a constant and is the size of the magnetic moment. For the matrix, N0= 8.49⫻1028 m−3 and Fe= 1.718 B at T = 550 ° C, resulting in
MAG= 3.94⫻1014 m−2 共Fe= 2.225 B at room temperature兲.32 For the nonmagnetic Cu precipitates, the
magnetic scattering length density is zero. The corresponding nuclear contrast is⌬NUC=Fe−Cu⬇N0FebcFe− N0CubcCu, where
N0 is the number density of atoms and bc the coherent scattering length 共bcFe= 9.45⫻10−15 m and b
c Cu= 7.72
⫻10−15 m兲. The density of the copper
precipitates depends on the stage in the structure evolution bcc→9R→3R→fcc. At the initial stage of the transforma-tion, coherent precipitates are formed 共N0Cu= N0Fe兲, resulting in ⌬NUC= 1.47⫻1014 m−2 共Fe= 8.02⫻1014 m−2 and
Cu= 6.55⫻1014 m−2兲. For the Fe-Cu-B-N alloy, nuclear and magnetic contrast is not significantly affected by the low concentration of added B and N. The same SANS measure-ments have also been performed on a high-purity Fe-B-N alloy 共0.046 wt % B, 0.039 wt % N, and 0.015 wt % Ce兲. The time evolution of the SANS signal revealed only a weak strain-dependent aging response corresponding to precipita-tion at dislocaprecipita-tions and interfaces. Potential reasons are:共1兲 the low solute concentrations of B an N and 共2兲 the weak scattering contrast between the Fe matrix and the BN pre-cipitates. For hexagonal BN the nuclear scattering length density amounts to BN= 7.75⫻1014 m−2, resulting in nuclear contrast of only⌬NUC=Fe−BN= 0.27⫻1014 m−2. For the less stable cubic BN values of BN = 12.3⫻1014 m−2 and ⌬
NUC=Fe−BN= −4.3⫻1014 m−2 are found.
As the magnetic scattering from the copper precipitates is dominant 关共⌬MAG兲2⬎共⌬NUC兲2兴, we have used the mag-netic component to estimate the phase fraction. For relatively small values, the volume fraction is estimated by fV⬵Q0,MAG/22共⌬MAG兲2. In Figs. 6共a兲 and6共b兲, the time evolution of the volume fraction of Cu precipitates, obtained by integrating the magnetic SANS component 共d⌺/d⍀兲MAGQ2 up to the maximum Q value共2.5 nm−1兲, is shown for the Fe-Cu and Fe-Cu-B-N alloys with 0%, 8%, and 24% prestrain.
For the Fe-Cu alloy 关Fig. 6共a兲兴, the precipitation in the initial aging stage 共⬍1 h兲 is accelerated in the deformed samples with respect to the undeformed sample. This accel-eration of the transformation kinetics can be explained by an increase in diffusion rate by fast pipe diffusion and an in-crease in potential nucleation sites. The dislocations gener-ated by deformation are expected to act as nucleation sites for the copper precipitates by decreasing the activation ergy for nucleation, most probably by a relief of strain en-ergy. In the later stages 共⬎2 h兲, the deformed Fe-Cu samples however approach a lower phase fraction of spheri-cal Cu precipitates than the undeformed sample.
For the Fe-Cu-B-N alloy关Fig.6共b兲兴, a strongly enhanced Cu precipitation in the undeformed sample is observed at the start of the aging compared to the undeformed Fe-Cu sample. The deformed Fe-Cu-B-N samples, on the other hand, show a slightly faster precipitation kinetics compared to the deformed Fe-Cu sample with the same prestrain. The fraction transformed after 12 h of aging at 550 ° C is nearly equal for the Fe-Cu alloys with and without added B and N. For both alloys, the fraction of nanoscale共spherical兲 precipi-tates reduces with the applied prestrain.
The equilibrium volume fraction of Cu precipitates is not expected to depend on the amount of prestrain. As shown in Figs.6共a兲and6共b兲, the volume fraction of the spherical pre-cipitates reached after 12 h of aging decreases however for increasing prestrain. This indicates that deformation either promotes Cu precipitation at dislocations and interfaces 共re-sulting in additional scattering at lower Q values兲 or reduces the growth rate of the precipitates. It is interesting to note that additional room-temperature SANS experiments on samples that were aged for 96 h at 550 ° C after applying a prestrain of 8% 共samples of Ref. 30兲 indicated a volume fraction of the spherical precipitates of 0.57% for Fe-Cu and 0.59% for Fe-Cu-B-N.
In the Q range of 0.2– 2 nm−1, the nuclear SANS com-ponent shows the same time evolution as the magnetic SANS component with a lower intensity, reflecting the precipitation of nanoscale 共spherical兲 Cu precipitates. As mentioned be-fore, in the low-Q region共⬍0.2 nm−1兲 an additional contri-bution to the nuclear scattering is observed that increases continuously with the aging time for the deformed samples. In order to monitor this additional contribution that reflects the precipitation of Cu along dislocations共and/or interfaces兲, we evaluated the time evolution of the nuclear scattering observed at low Q.
Experimentally, the nuclear scattered intensity 共d⌺/d⍀兲 at low Q values共⬍0.2 nm−1兲 is described by a power law of the form
共d⌺/d⍀兲 = AQn
+ B, 共5兲
where n is the exponent and A the coefficient of the power law while B corresponds to the background共due to incoher-ent scattering and diffuse coherincoher-ent scattering兲. Within the experimental resolution, the exponent is found to be equal to n = −4 throughout the whole aging process for all the Fe-Cu and Fe-Cu-B-N samples with and without prestrain. For the homogenized sample, the Q−4 power-law behavior of the SANS signal at low Q originates from scattering of grain
boundaries. The increase in the size of the Q−4 power-law amplitude suggests Cu precipitation at dislocations共or inter-faces兲.
Recently, the small-angle scattering from dislocations was analyzed in detail by Long and co-workers.33,34It was found
that the strain fields associated with the dislocations give rise to a nuclear small-angle scattering signal in the form of a Q−2 power law for dislocation cores, Q−3 for dislocation dipoles and Q−4共1−2Q−2兲 for dislocation walls. In the low-Q range the scattering from dislocation walls will be dominant. For finite thickness walls with sharp boundaries 共= 0兲 the Q behavior becomes Q−4. This prediction is in agreement with our experimental data. For magnetic scattering it is predicted35 that the nuclear scattering term is multiplied by
共Q2+ Q m
2兲−2, where 1/Qm is a characteristic magnetic scale for magnetostatic field variations. For QⰆQm the magnetic and nuclear scattering show the same Q−4 power law, as we found experimentally.
In Figs.6共c兲and6共d兲, the time evolution of the coefficient A of the Q−4power law during aging is shown for the Fe-Cu and Fe-Cu-B-N alloys with 0%, 8%, and 24% prestrain. For the Fe-Cu alloy 关Fig. 6共c兲兴, no significant increase in A is observed in the undeformed sample during aging while the predeformed samples show a strong increase with aging time. This strongly suggests that a significant fraction of the
nuclear scattering at low-Q values originates from a network of Cu atoms or clusters decorating the existing dislocations 共or interfaces兲. The aging curves of A for the two deformed samples are close to each other but the most severely de-formed sample with 24% prestrain exhibits the highest A value at all times. This means that the contribution from the network of Cu along dislocations 共or interfaces兲 increases with the applied level of prestrain due to higher density of dislocations before aging. For the Fe-Cu-B-N alloy 关Fig. 6共d兲兴, only a very weak aging response is observed for A, with a slight increase for higher prestrains. The suppression of the aging response of A in the deformed Fe-Cu-B-N samples probably originates from a full decoration of the dislocations and interfaces by mobile N and/or B atoms be-fore the less mobile Cu atoms have had the chance to pre-cipitate at these sites.
It is important to note that the annealing response of the Q−4 power-law contribution in the nuclear scattering at low Q is considered to be related to the contrast in scattering length density of the Cu segregated at the dislocation walls and not due to a modification of the strain fields itself. This interpretation is confirmed by a comparison of the as-quenched samples with and without prestrain before aging. For these samples, which contain dislocations but no Cu precipitates, no significant enhancement in the low
FIG. 6. 共Color online兲 Time evolution of the volume fraction fVfor共a兲 the Fe-Cu alloy and 共b兲 the Fe-Cu-B-N alloy with 0%, 8%, and 24% prestrain, derived from the magnetic SANS component shown during aging at 550 ° C. For comparison, the time evolution of the coefficient A of the Q−4power law is shown for共c兲 the Fe-Cu alloy and 共d兲 the Fe-Cu-B-N alloy with 0%, 8%, and 24% prestrain, derived from nuclear SANS component around Q = 0.1 nm−1during aging at 550 ° C. The inset in Fig.6共a兲shows the early aging stage up to 1.2 h.
Q共⬍0.2 nm−1兲 part of the nuclear scattering is observed. The increase in the coefficient A, caused by Cu precipita-tion at dislocaprecipita-tions, is expected to scale with the contrast in scattering length density. For nuclear scattering, the scatter-ing contrast 共⌬兲2 originates from the difference in nuclear scattering length density of the alloy matrixm and the cop-per precipitatep. For comparison the value of A/2共⌬兲2, which is proportional to the phase fraction of Cu precipita-tion at dislocaprecipita-tions, is also shown in Fig.6.
The increase in coefficient A for increasing prestrain 关Figs. 6共c兲 and6共d兲兴 shows an inverse correlation with the volume fraction of spherical precipitates 关Figs. 6共a兲 and 6共b兲兴. For the Fe-Cu-B-N alloys the signal of the copper precipitation at dislocations is much weaker than for the Fe-Cu alloys. A possible cause for this may be a reduced scattering contrast 共⌬兲2 when Cu precipitates in combina-tion with B and/or N at dislocacombina-tions and interfaces.
Now that we have established the main contributions to the SANS signal, we can analyze the time evolution of the precipitate size distribution in detail. As discussed above, the neutron scattering from a ferromagnetic material共iron-based alloy兲 containing nonmagnetic particles with a different chemical composition 共Cu-rich precipitates兲 generally con-tains both magnetic scattering and nuclear scattering compo-nents. The magnetic scattering originates from a difference in magnetization and the nuclear scattering from a difference in chemical composition. By applying a strong magnetic field to the specimen, these two components could be separated.15,16For a dilute system of particles embedded in a
homogeneous matrix, the macroscopic differential scattering cross section 共d⌺/d⍀兲 characterizes the scattering power by16,36
where ⌬=p−m is the difference in the scattering length density of the precipitatepand the matrixm. The strength of the magnetic 共nuclear兲 scattering is directly proportional to the magnetic 共nuclear兲 contrast 共⌬兲2. For spherical precipitates with a radius R, the particle volume is V共R兲=4R3/3 and the form factor is F共Q,R兲 = 3关sin共QR兲−共QR兲cos共QR兲兴/共QR兲3. DN共R兲 is the size distri-bution function for the number of precipitates per unit vol-ume. This number distribution DN共R兲 is directly related to the volume distribution DV共R兲=V共R兲DN共R兲. Integration of DN共R兲 gives the number of precipitates per unit volume Np while integration of DV共R兲 results in the volume phase frac-tion of the precipitates fV.
In order to relate the scattering curves of the SANS ex-periments to the size distribution of the precipitates, some model assumptions have to be made. From previous TEM observations,28 we know that the spherical Cu precipitates
approximately show a log-normal size distribution DN共R兲 which is described by DN共R兲 = NP R
再− 关ln共R兲 − ln共Rm兲兴2 22
where NP is the number density of precipitates, Rm is the median radius, and the standard deviation of the size dis-tribution.
Figure 7 shows the log-normal volume distribution DV共=DNV兲 of spherical Cu precipitates with precipitate ra-dius R as a function of the aging time for the Fe-Cu and Fe-Cu-B-N alloys with 0%, 8%, and 24% prestrain. The par-ticle size distributions were obtained by a fit of the magnetic SANS component with a log-normal distribution using the
SASFIT program.37 For short aging times 共⬍1 h兲, the peak
height of the volume distribution increases with the aging time without changing the peak position, indicating that nucleation is the dominant process in the very early aging stage. For longer aging times, the volume distribution of the Cu precipitates broadens, the peak height reduces and the peak position increases with aging time, suggesting that the growth of precipitates is the dominant process.
In Fig.8, the time evolution of the median radius Rmand the number density NPof the nanoscale precipitates is shown for the Fe-Cu and Fe-Cu-B-N alloys with 0%, 8%, and 24% prestrain during aging. The values of Rm and Np follow di-rectly from the fit关Npis obtained by integration of the num-ber distribution DN共R兲兴. The mean radius Rm of spherical precipitates 关Figs. 8共a兲 and8共b兲兴 initially increases roughly linearly with time under the influence of continuous nucle-ation and growth of the precipitates. In the later stages, the growth of the spherical precipitates closely follows a power law of the form Rm= ct1/3, with a growth constant c that decreases with increasing prestrain. This power-law behavior is representative for coarsening of nucleated precipitates.44,38
The decrease in c, observed for increasing prestrain, is prob-ably due to the competing precipitation at dislocations and interfaces, which reduces the potential growth of spherical precipitates within the matrix. The number density Np关Figs. 8共c兲and8共d兲兴 rises rapidly to a very high level in the nucle-ation stage and subsequently decreases gradually during ag-ing. The corresponding interparticle distance Lp⬀1/Np
1/3, on the other hand, gradually becomes larger for increasing aging time. This indicates that the growth of larger particles occurs at the expense of smaller particles.
C. Transmission electron microscopy
As shown in Fig.9共a兲, for the undeformed Fe-Cu sample a limited number of larger Cu particles and few dislocations are observed in the TEM bright-field images after aging at 550 ° C for 12 h. In Figs.9共b兲and9共c兲, the TEM bright-field images are shown for the Fe-Cu sample with 8% prestrain after aging at 550 ° C for 12 h. Copper precipitation is found as isolated particles within the matrix, as particles at pre-existing dislocations and as a Cu decorated network of dis-locations and/or interfaces. The existence of twinned 9R par-ticles共with a diameter of 6 nm兲 was confirmed in the studied Fe-Cu alloy by HREM关see Fig.9共e兲兴.
For the deformed Fe-Cu alloy, the Cu particles are pref-erentially formed on dislocations. Only a few particles are found to be larger than 30 nm in diameter and therefore, judged on their size, may have transformed to the equilib-rium fcc lattice structure.
From traditional TEM images, only the Cu particles with a diameter bigger than 5 nm 共critical size for the bcc→9R transition兲 are distinguishable. Because the smaller particles
are coherent with the matrix共with the same bcc crystal struc-ture兲 and the difference of mass density between Cu and Fe is low, the contrast of these smallest particles is poor.
Comparing Figs.9共a兲and9共b兲to Fig.9共c兲, it can be seen that there are more distinguishable precipitates in the 8% prestrained sample than in the undeformed sample. More-over, the distinguishable Cu particles are predominantly
con-nected to heterogeneously distributed residual dislocations. In between the precipitates, dislocation-free regions are ob-served, where larger particles do not exist.
In Fig. 9共d兲, a TEM bright-field image for the 8% de-formed Fe-Cu-B-N sample with 12 h aging at 550 ° C is shown. Again, spherical Cu precipitates and dislocations are observed. However, compared to the Fe-Cu sample, fewer
FIG. 7. 共Color online兲 Volume distribution DVof spherical Cu precipitates in共a兲–共c兲 the Fe-Cu alloy and 共d兲–共f兲 the Fe-Cu-B-N alloy with 0%, 8%, and 24% prestrain during aging at 550 ° C. DVis derived from a fit of the time-resolved magnetic SANS data共see text兲.
copper precipitates are connected to the dislocations 共or in-terfaces兲 and more are observed isolated in the matrix.
IV. DISCUSSION A. Precipitation kinetics
The precipitation kinetics for Cu segregation in the ho-mogenized Fe-Cu alloys shown in Fig. 7 is controlled by three different processes:共i兲 nucleation, 共ii兲 growth and 共iii兲 coarsening.13In the early-stage precipitation, Cu precipitates
nucleate and subsequently grow in the homogenized matrix. As the phase fraction of precipitated Cu is small in the early stages, the homogenized matrix shows a high supersaturation of solute Cu. The growth of nucleated Cu precipitates ini-tially shows no interaction with other precipitates. In this case the growth is described by the Zener model,40 which
predicts that the particle radius scales as R⬀t1/2. When a significant phase fraction of Cu precipitates has formed then nucleation stops as the supersaturation of solute Cu is sig-nificantly lowered. At this stage the growth of individual precipitates becomes strongly correlated and is controlled by a coarsening process where the larger precipitates grow at the expense of the smaller precipitates that disappear.
Since dislocations act as fast pipe-diffusion paths and as heterogeneous nucleation sites, the precipitation kinetics is strongly affected by the dislocation structure. It has been found that dislocations are arranged in ordered patterns, con-sisting of dislocation cells and dislocation-free regions, dur-ing plastic deformation of Fe-Cu alloys41 and pure copper.42
The Cu particles located at dislocations and at the dislocation network, observed in Figs. 9共b兲 and9共c兲 clearly signal the close interaction of Cu precipitation and dislocations during aging. The dislocation structure will generally vary with the deformation mode, strain level, and strain rate.41,43,39
In the early-stage precipitation regime 共⬍4 h兲 copper precipitation at dislocations is strongly promoted by the pre-strain in the Fe-Cu alloy. When N and/or B are added to the alloy, we see that the precipitation of copper at dislocations is largely suppressed. This is probably caused by the fast diffusion of mobile N and/or B to dislocations. A saturation with N and/or B effectively blocks Cu precipitation at dislo-cations. It is remarkable that the undeformed Fe-Cu-B-N sample has the fastest Cu precipitation kinetics of all the Fe-Cu and Fe-Cu-B-N samples. A possible explanation is that the nucleation barrier for copper precipitation in the ma-trix is lowered by the solute N and/or B. In the prestrained samples, a significant part of the solute N and/or B may have
0 2 4 6 8 10 12 1017 1018 1019 1020 24% pre-strain 8% pre-strain 0% pre-strain NP (cm -3 ) Aging Time (h) Fe-Cu T = 550oC
(c)0 2 4 6 8 10 12 0 1 2 3 Fe-Cu T = 550oC 0% pre-strain 8% pre-strain 24% pre-strain Rm (n m) Aging Time (h)
(a)0 2 4 6 8 10 12 0 1 2 3 Fe-Cu-B-N T = 550oC 0% pre-strain 8% pre-strain 24% pre-strain Rm (n m) Aging Time (h)
(b)0 2 4 6 8 10 12 1017 1018 1019 1020 24% pre-strain 8% pre-strain 0% pre-strain NP (c m -3 ) Aging Time (h) Fe-Cu-B-N T = 550oC
FIG. 8.共Color online兲 Time evolution of the median radius Rmand the number density NPof spherical Cu precipitates in the Fe-Cu alloy and the Fe-Cu-B-N alloy with 0%, 8%, and 24% prestrain, derived from the magnetic SANS component during aging at 550 ° C共see text兲.
preferentially segregated at dislocations, reducing the nucle-ation rate of Cu precipitates within the matrix.
In the later stages of aging共⬎4 h兲, the Cu concentration in the matrix is considerably reduced and the size evolution of the spherical nanoscale Cu precipitates is controlled by a coarsening of the formed precipitates. The growth of the pre-cipitates during further aging is then described by the Lifshitz-Slyozov-Wagner共LSW兲 theory44,38
Rm3 = Kt, 共8兲
where Rmis the average radius of the precipitate. The devia-tions from the R3 law, observed in the initial aging stage, originate from the simultaneous nucleation and growth pro-cesses. The LSW theory for coarsening with volume diffu-sion control for small volume fractions of spherical particles predicts the proportionality constant is given by
K =8D⌫C⬁⍀ 2
T exp共− Q/kT兲, 共9兲
where D = 1.6⫻10−18 m2/s is the bulk diffusion coefficient of Cu in ␣-Fe at 550 ° C,45 ⌫=0.58 J/m2 is the interfacial
energy between Cu and Fe,46 C
⬁= 0.18 at. % the solubility limit of Cu in Fe at 550 ° C,47⍀=1.18⫻10−29 m3/atom the atomic volume of solute in the dispersed phase, Q the acti-vation energy of bulk Cu diffusion in Fe, k Boltzmann’s constant, and T temperature. For the Fe-Cu alloy, the experi-mental value of the proportionality constant at 550 ° C amounts to K0%= 2.9⫻10−31 m3/s for the undeformed sample, which is significantly lower than the value of K = 9.4⫻10−31 m3/s reported by Monzen and co-workers at a temperature of 650 ° C.46 The experimental values
of K8%= 2.6⫻10−31 m3/s for 8% prestrain and K24%= 1.9⫻10−31 m3/s for 24% prestrain indicate that the growth rates for spherical Cu particles in the matrix de-creases with increasing dislocation densities. The lower growth rates of the predeformed samples may be related to the reduced Cu concentration in dislocation-free regions due to the segregation of Cu at dislocations.
When we compare the volume fraction of Cu occupied by the spherical nanoscale precipitates after 12 h aging at 550 ° C, we see that about half of the nominal copper con-centration has formed precipitates for both the Fe-Cu and Fe-Cu-B-N samples. With increasing prestrain, a slight de-crease in the precipitated volume fraction is observed for both alloys. In SAXS measurements on deformed Fe-Cu alloys,28it was reported that the volume fraction of Cu pre-cipitates increases faster in the predeformed sample than in the undeformed sample but saturates at the same value for long aging times up to 300 h at 500 ° C. They claimed that in peak-hardness condition the Fe-Cu alloy has not reach a complete precipitation and the volume fraction of precipi-tates reaches about 48% and 52% of equilibrium value for the undeformed and deformed samples.
B. Structure evolution of the precipitates
Experimentally, it was found that in binary Fe-Cu alloys the structure evolution of Cu precipitates follows the se-quence bcc→9R→3R→fcc.7,48It is believed that the
struc-ture changes in the Cu precipitates is triggered by a critical size and driven by minimizing the interfacial strain energy. The volume strain energy within the Cu precipitate is rela-tively weak because the difference in atomic radii of Fe and Cu is small共3%兲. When the nucleated coherent bcc clusters grow in size they transform into the 9R structure beyond a critical size of 4–6 nm in diameter, followed by the transfor-mation from the 9R structure to the 3R or fcc structure at a critical size of 15–17 nm in diameter.
Using the fitted particle size distributions for the spherical nanoscale Cu precipitates of Fig.7, we can now, based on the reported critical sizes, estimate what fraction of the formed precipitates has a bcc structure, 9R structure or 3R/fcc struc-ture. The volume fraction is now directly obtained by inte-gration of the volume distribution DV共R兲 while the number fraction is obtained by integration of the number distribution DN共R兲. Figure10shows the estimated evolution of the rela-tive volume and number fraction of the Cu precipitates in the Fe-Cu and Fe-Cu-B-N alloys during aging at 550 ° C. For this evaluation, we have used a critical radius of Rbcc→9R= 2.5 nm for the transition from the bcc structure to
FIG. 9. TEM images of共a兲 the undeformed Fe-Cu alloy and 共b兲 and 共c兲 the Fe-Cu alloy with 8% prestrain and 共d兲 the Fe-Cu-B-N alloy with 8% prestrain after aging at 550 ° C for 12 h. In the undeformed sample共a兲 randomly distributed spherical Cu precipi-tates are observed. In the deformed samples共b兲–共d兲 the dislocations are decorated with Cu precipitates. The Fe-Cu alloy with 8% pre-strain 共c兲 shows a network composed of dislocations and precipi-tates. In共e兲 the existence of twinned 9R particles in the Fe-Cu alloy was confirmed by high resolution electron microscopy共HREM兲.
the 9R structure and a critical radius of R9R→3R/fcc= 8 nm for the transition from the 9R structure to the 3R or fcc structure. In this evaluation we have assumed that the structural changes are purely determined by the size of the precipitate as the structure itself is not probed in the SANS measure-ments.
For the Fe-Cu alloy, prestrain accelerates the transition from the coherent bcc structure to the incoherent 9R while for the Fe-Cu-B-N alloy prestrain delays the formation of the 9R structure. Within 12 h of aging at 550 ° C, only a minor fraction of the copper precipitates have reached a size corre-sponding to the 3R or fcc structure. The prestrain slightly promotes the 9R→3R or fcc transformation for both the alloys. It is noted that in peak-hardness condition, which was reached after an aging time of about 6 h for Fe-Cu and about 4 h for Fe-Cu-B-N, the undeformed samples show a domi-nant phase fraction with the 9R structure, while for the de-formed samples equal phase fractions of about 50% are found for the bcc and 9R structure. For the Fe-Cu sample with 8% prestrain, a significant fraction of semicoherent pre-cipitates with a 9R structure forms after about 1 h. This is consistent with earlier positron annihilation spectroscopy measurements on the same material.30
C. Self-healing of defects
In previous studies on austenitic stainless steels, it was found that the addition of B with N and Cu both lead to a significant increase in the creep lifetime at high temperatures.2,3The improved creep lifetime was ascribed to
a self-healing of nucleated creep cavities by the formation of BN and/or Cu precipitates. Here we have systematically studied the aging behavior of prestrained high-purity Fe-Cu and Fe-Cu-B-N alloys by time-resolved SANS measure-ments at a temperature of 550 ° C. From the observed cipitation kinetics, we have evaluated the influence of pre-strain and added B and N on the precipitation kinetics of Cu. For the Fe-Cu alloy, Cu has a strong tendency to segregate at open volume defects such as dislocations, which is expected to be very beneficial for self-healing of creep cavities. Simul-taneously, copper is also precipitating within the matrix which leads to a precipitation strengthening of the alloy 共un-til peak aging is reached兲. For the Fe-Cu-B-N alloy, the ad-dition of boron and nitrogen accelerates the formation of spherical Cu precipitates within the matrix, but strongly re-duces the Cu precipitation along dislocations in the deformed samples. Both effects are probably caused by a fast segrega-tion of the mobile B and N atoms along dislocasegrega-tions,
FIG. 10. 共Color online兲 Time evolution of the fractional contributions of Cu precipitates with a bcc 共solid兲, 9R 共half solid兲, and 3R and fcc共open兲 structure for the Fe-Cu alloys with 0% 共square兲, 8% 共circle兲, and 24% 共triangle兲 prestrain during aging at 550 °C. The fractional contributions are obtained from the experimental particle size distributions.
venting Cu precipitation along these dislocations, but pro-moting the nucleation of nanoscale Cu precipitates in dislocation-free regions. The enhanced nucleation of nano-scale Cu precipitates is either due to the effect of remnant B and N or the lower loss in Cu for the dislocation-free re-gions, compared to the Fe-Cu alloy with the same prestrain. One therefore expects that in Fe-Cu-B-N alloys self-healing of small defects will initially take place by the formation of BN precipitates, and may be assisted by copper precipitation when larger creep cavities are formed.
We have performed time-resolved SANS measurements during isothermal aging at a temperature of 550 ° C in order to study the influence of tensile deformation on the precipi-tation kinetics of copper in a high-purity Fe-Cu and Fe-Cu-B-N alloys. The time evolution of the precipitate size distri-bution was monitored at high temperatures for copper solutionised samples with 0%, 8%, and 24% strain applied by prior tensile deformation. Complementary TEM measure-ments were performed on the aged samples to characterize the formed precipitates. The mechanical behavior was evalu-ated by hardness tests as a function of aging time. The main conclusions derived from these experiments are: 共1兲 the SANS signal of the Fe-Cu and Fe-Cu-B-N alloys indicate that the precipitation of copper occurs in the form of 共a兲 spherical nanoscale precipitates within the grains and 共b兲 decoration of dislocations and/or interfaces. Both contribu-tions were monitored independently as a function of aging time.
共2兲 For the Fe-Cu alloy, the presence of dislocations re-sulting from the prestrain promotes the nucleation of
spheri-cal nanosspheri-cale precipitates whereas the growth seems to be retarded. The precipitation of Cu along dislocations is strongly promoted by increasing levels of prestrain.
共3兲 For the Fe-Cu-B-N alloy, the addition of boron and nitrogen accelerates the formation of spherical nanoscale Cu precipitates and strongly reduces the Cu precipitation along dislocations in deformed samples. Both effects are probably caused by a fast segregation of the mobile B and N atoms along dislocations, preventing Cu precipitation along these dislocations, but promoting the nucleation of nanoscale Cu precipitates. One therefore expects that in Fe-Cu-B-N alloys self-healing of small defects will initially take place by the formation of BN precipitates.
共4兲 The experimental time evolution of the particle size distribution for spherical nanoscale copper precipitates gives a direct estimate of the fraction of copper precipitates with a coherent bcc structure, a 3R structure, and a 9R or fcc struc-ture. The transition from coherent to partially incoherent Cu clusters is in good agreement with recent positron annihila-tion spectroscopy results.30
This research project has been financially supported by the Innovation-Oriented research Program on self-healing materials 共IOP under Project No. SHM0636兲 of the Dutch Ministry of Economic Affairs and by the European Commis-sion under the Seventh Framework Programme through the “Research Infrastructures” action of the “Capacities” Pro-gramme, Contracts No. CP-CSA_INFRA-2008-1.1.1 and No. 226507-NMI3. The authors are very grateful to Shirish Chodankar and Agnieszka Wilk for assistance with the SANS experiments and Marcel Sluiter for fruitful discus-sions.
*Corresponding author. FAX: ⫹31共0兲152788303;
1R. N. Lumley, A. J. Morton, and I. J. Polmear,Acta Mater. 50, 3597共2002兲.
2K. Laha, J. Kyono, S. Kishimoto, and N. Shinya,Scr. Mater. 52, 675共2005兲.
3K. Laha, J. Kyono, and N. Shinya,Scr. Mater. 56, 915共2007兲. 4Self-Healing Materials: An Alternative Approach to 20 Centuries
of Materials Science, Springer Series in Materials Science Vol. 100, edited by S. van der Zwaag共Springer, Dordrecht, 2007兲. 5U. Dahmen, P. Ferguson, and K. H. Westmacott, Acta Metall.
6P. J. Othen, M. L. Jenkins, G. D. W. Smith, and W. J. Phythian, Philos. Mag. Lett. 64, 383共1991兲.
7P. J. Othen, M. L. Jenkins, and G. D. W. Smith,Philos. Mag. A 70, 1共1994兲.
8R. Monzen, M. L. Jenkins, and A. P. Sutton,Philos. Mag. A 80, 711共2000兲.
9M. K. Miller, P. Pareige, and M. G. Burke,Mater. Charact. 44, 235共2000兲.
10P. Pareige, K. F. Russell, and M. K. Miller, Appl. Surf. Sci. 94-95, 362共1996兲.
11P. Pareige and M. K. Miller,Appl. Surf. Sci. 94-95, 370共1996兲. 12D. Isheim, M. S. Gagliano, M. E. Fine, and D. N. Seidman,Acta
Mater. 54, 841共2006兲.
13R. Kampmann and R. Wagner, in Atomic Transport and Defects in Metals by Neutron Scattering, edited by C. Janot, W. Petry, D. Richter, and T. Springer共Springer-Verlag, Berlin, 1986兲, p. 73. 14G. M. Worrall, J. T. Buswell, C. A. English, M. G. Hetherington,
and G. D. W. Smith,J. Nucl. Mater. 148, 107共1987兲.
15K. Osamura, H. Okuda, M. Takashima, K. Asano, and M. Furu-saka, Mater. Trans., JIM 34, 305共1993兲.
16K. Osamura, H. Okuda, S. Ochiai, M. Takashima, K. Asano, M. Furusaka, K. Kishida, and F. Kurosawa, ISIJ Int. 34, 359 共1994兲.
17Y. Nagai, M. Hasegawa, Z. Tang, A. Hempel, K. Yubuta, T. Shimamura, Y. Kawazoe, A. Kawai, and F. Kano,Phys. Rev. B
18Y. Nagai, T. Chiba, Z. Tang, T. Akahane, T. Kanai, M. Hase-gawa, M. Takenaka, and E. Kuramoto, Phys. Rev. Lett. 87, 176402共2001兲.
19K. Sumiyama, Y. Yoshitake, and Y. Nakamura,Acta Metall. 33, 1785共1985兲.
R. Odette,Philos. Mag. Lett. 82, 609共2002兲.
21J. J. Blackstock and G. J. Ackland, Philos. Mag. A 81, 2127 共2001兲.
22Y. Le Bouar,Acta Mater. 49, 2661共2001兲.
23J.-H. Shim, Y. W. Cho, S. C. Kwon, W. W. Kim, and B. D. Wirth, Appl. Phys. Lett. 90, 021906共2007兲.
24E. Kozeschnik,Scr. Mater. 59, 1018共2008兲.
25M. Legros, G. Dehm, E. Arzt, and T. J. Balk,Science 319, 1646 共2008兲.
26C. Zhang, M. Enomoto, T. Yamashita, and N. Sano, Metall. Mater. Trans. A 35, 1263共2004兲.
27K. Osamura, H. Okuda, K. Asano, M. Furusaka, K. Kishida, F. Kurosawa, and R. Uemori,ISIJ Int. 34, 346共1994兲.
28A. Deschamps, M. Militzer, and W. J. Poole,ISIJ Int. 41, 196 共2001兲.
29A. Deschamps, M. Militzer, and W. J. Poole,ISIJ Int. 43, 1826 共2003兲.
30S. M. He, N. H. van Dijk, H. Schut, E. R. Peekstok, and S. van der Zwaag,Phys. Rev. B 81, 094103共2010兲.
31A. Wiedenmann, in Neutron Scattering from Magnetic Materials, edited by T. Chatterji共Elsevier, Amsterdam, 2006兲, p. 473. 32A. S. Arrott and B. Heinrich,J. Appl. Phys. 52, 2113共1981兲. 33G. G. Long and L. E. Levine,Acta Crystallogr., Sect. A: Found.
Crystallogr. 61, 557共2005兲.
34R. Thomson, L. E. Levine, and G. G. Long,Acta Crystallogr., Sect. A: Found. Crystallogr. 55, 433共1999兲.
35W. Schmatz, T. Springer, J. Schelten, and K. Ibel,J. Appl. Crys-tallogr. 7, 96共1974兲.
36N. H. van Dijk, W. G. Bouwman, S. E. Offerman, M. Th. Re-kveldt, J. Sietsma, S. van der Zwaag, A. Bodin, and R. K. Heenan,Metall. Mater. Trans. A 33, 1883共2002兲.
37J. Kohlbrecher and I. Bressler,SASFIT: software package for fit-ting small-angle scattering curves, http://kur.web.psi.ch/sans1/ SANSSoft/sasfit.html
38I. M. Lifshitz and V. V. Slyozov, J. Phys. Chem. Solids 19, 35 共1961兲.
39C. Wagner, Z. Elektrochem. 65, 581共1961兲. 40C. Zener,J. Appl. Phys. 20, 950共1949兲.
41T. Ishizaki, T. Yoshiie, K. Sato, S. Yanagita, Q. Xu, M. Komatsu, and M. Kiritan,Mater. Sci. Eng., A 350, 102共2003兲.
42B. Jakobsen, H. F. Poulsen, U. Lienert, J. Almer, S. D. Shastri, H. O. Sørensen, C. Gundlach, and W. Pantleon, Science 312, 889共2006兲.
43K. Sato, M. Kai, K. Mitoma, Q. Xu, and T. Yoshiie,Phys. Status Solidi C 4, 3559共2007兲.
44D. Hughes, D. C. Chrzan, Q. Liu, and N. Hansen,Acta Mater. 45, 105共1997兲.
45M. Perez, M. Dumont, and D. Acevedo-Reyes,Acta Mater. 56, 2119共2008兲.
46R. Monzen, K. Takada, and C. Watanabe, ISIJ Int. 44, 442 共2004兲.
47M. Perez, F. Perrard, V. Massardier, X. Kleber, A. Deschamps, H. De Monestrol, P. Pareige, and G. Covarel,Philos. Mag. 85, 2197共2005兲.